The Use of Polarizable [AuX2(CN)2]- (X = Br, I) Building Blocks Toward the Formation of Birefringent Coordination Polymers
Jeffrey S. Ovens; Andrew R. Geisheimer; Alexei A. Bokov; Zuo-Guang Ye; Daniel B. Leznoff; Inorganic Chemistry 49 (2010) 9609–9616; doi:10.1021/ic101357y

data_4316834
_publ_contact_author_address
; 
Leznoff, Daniel B.
Department of Chemistry
Simon Fraser University
Burnaby, British Columbia
Canada         V5A 1S6
;
_publ_contact_author_email       dleznoff@sfu.ca
_publ_contact_author_fax         +1-778-782-3765
_publ_contact_author_name        'Daniel B. Leznoff'
_publ_contact_author_phone       +1-778-782-4887
_publ_section_title
;
 The Use of Polarizable [AuX2(CN)2]- (X = Br, I) Building Blocks Toward
 the Formation of Birefringent Coordination Polymers
;
_journal_name_full               'Inorganic Chemistry'
_journal_page_first              9609
_journal_page_last               9616
_journal_paper_doi               10.1021/ic101357y
_journal_volume                  49
_journal_year                    2010
_chemical_formula_moiety         'C34 H22 Au2 Br4 N10 Ni1'
_chemical_formula_sum            'C34 H22 Au2 Br4 N10 Ni'
_chemical_formula_weight         1342.88
_chemical_name_systematic        ?
_space_group_IT_number           2
_symmetry_cell_setting           triclinic
_symmetry_space_group_name_Hall  '-P 1'
_symmetry_space_group_name_H-M   'P -1'
_atom_sites_solution_hydrogens   geom
_atom_sites_solution_primary     direct
_cell_angle_alpha                118.012(2)
_cell_angle_beta                 97.324(3)
_cell_angle_gamma                92.434(2)
_cell_formula_units_Z            2
_cell_length_a                   12.556(4)
_cell_length_b                   13.072(2)
_cell_length_c                   13.472(2)
_cell_measurement_reflns_used    9909
_cell_measurement_temperature    296(2)
_cell_measurement_theta_max      28.331
_cell_measurement_theta_min      1.737
_cell_volume                     1922.9(7)
_computing_cell_refinement       'Bruker SAINT'
_computing_data_collection       'Bruker APEX2'
_computing_data_reduction        'Bruker SAINT'
_computing_structure_solution
; 
SIR92 (Altomare et al, 1994)
CRYSTALS (Watkin, 1988) 
;
_diffrn_ambient_temperature      293
_diffrn_measured_fraction_theta_full 0.996
_diffrn_measured_fraction_theta_max 0.917
_diffrn_measurement_device_type  'Bruker APEX-II CCD'
_diffrn_measurement_method       '\w scans'
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.035
_diffrn_reflns_limit_h_max       16
_diffrn_reflns_limit_h_min       -15
_diffrn_reflns_limit_k_max       17
_diffrn_reflns_limit_k_min       -17
_diffrn_reflns_limit_l_max       17
_diffrn_reflns_limit_l_min       -17
_diffrn_reflns_number            22191
_diffrn_reflns_theta_full        25.781
_diffrn_reflns_theta_max         28.331
_diffrn_reflns_theta_min         1.737
_exptl_absorpt_coefficient_mu    12.291
_exptl_absorpt_correction_T_max  0.7457
_exptl_absorpt_correction_T_min  0.4379
_exptl_absorpt_correction_type   multi-scan
_exptl_crystal_colour            orange
_exptl_crystal_density_diffrn    2.319
_exptl_crystal_description       block
_exptl_crystal_F_000             1244
_exptl_crystal_size_max          0.35
_exptl_crystal_size_mid          0.31
_exptl_crystal_size_min          0.27
_refine_diff_density_max         1.83
_refine_diff_density_min         -1.93
_refine_ls_extinction_coef       3.3(17)
_refine_ls_extinction_method     'Larson (1970), Equation 22'
_refine_ls_goodness_of_fit_ref   1.0283
_refine_ls_hydrogen_treatment    none
_refine_ls_matrix_type           full
_refine_ls_number_parameters     445
_refine_ls_number_reflns         5723
_refine_ls_number_restraints     8
_refine_ls_R_factor_all          0.0622
_refine_ls_R_factor_gt           0.0370
_refine_ls_shift/su_max          0.0016105
_refine_ls_structure_factor_coef F
_refine_ls_weighting_details
;
 Method= Modified Sheldrick 
 w=1/[\s^2^(F) + ( 0.00P)^2^ + 0.10P] 
 ,where P=(max(Fo,0) + 2Fc)/3 
;
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_all         0.0726
_refine_ls_wR_factor_gt          0.0487
_refine_ls_wR_factor_ref         0.0482
_reflns_limit_h_max              15
_reflns_limit_h_min              -16
_reflns_limit_k_max              15
_reflns_limit_k_min              -17
_reflns_limit_l_max              17
_reflns_limit_l_min              0
_reflns_number_gt                5903
_reflns_number_total             8793
_reflns_threshold_expression     I>2.0\s(I)
_oxford_diffrn_Wilson_B_factor   3.61
_oxford_diffrn_Wilson_scale      675.58
_oxford_refine_ls_r_factor_ref   0.0359
_oxford_refine_ls_scale          0.05939(9)
_oxford_reflns_number_all        8793
_oxford_reflns_threshold_expression_ref I>2.5\s(I)
_cod_data_source_file            ic101357y_si_001_6.cif
_cod_data_source_block           NiTerpy
_cod_depositor_comments
;
The following automatic conversions were performed:

'_symmetry_cell_setting' value 'Triclinic' changed to 'triclinic'
according to the built-in table from CIF Core dictionary named
'cif_core.dic' version 2.4.1 from
2010-06-29.

'_exptl_absorpt_correction_type' value 'Multi-scan'
changed to 'multi-scan' according to the built-in table from CIF Core
dictionary named 'cif_core.dic' version 2.4.1 from 2010-06-29.

Automatic conversion script
Id: cif_fix_values 1646 2011-03-28 12:23:43Z adriana 
;
_cod_original_cell_volume        1922.9(8)
_cod_original_formula_sum        'C34 H22 Au2 Br4 N10 Ni1'
_cod_database_code               4316834